Measurement of valence-band offset at native
oxide/BaSi2 interfaces by hard x-ray
Takabe Ryota, Du Weijie, Ito Keita, Takeuchi
Hiroki, Toko Kaoru, Ueda Shigenori, Kimura
Akio, Suemasu Takashi
Journal of applied physics
(C) 2016 AIP Publishing LLC.
This article may be downloaded for personal
use only. Any other use requires prior
permission of the author and the American
Institute of Physics.The following article
appeared in J. Appl. Phys. 119, 025306 (2016)
and may be found at
Measurement of valence-band offset at native oxide/BaSi2
interfaces by hard
x-ray photoelectron spectroscopy
Institute of Applied Physics, University of Tsukuba, Tsukuba, Ibaraki 305-8573, Japan
Japan Society for the Promotion of Science (JSPS), Chiyoda, Tokyo 102-0083, Japan
Department of Electronic Engineering, Graduate School of Engineering, Tohoku University, Sendai 980-8579, Japan
Synchrotron X-ray Station at SPring-8, National Institute for Materials Science (NIMS), Hyogo 679-5148, Japan
Quantum Beam Unit, NIMS, Tsukuba, Ibaraki 305-0047, Japan
Graduate School of Science, Hiroshima University, Higashi-hiroshima 739-8526, Japan
Japan Science and Technology Agency, CREST, Tokyo 102-0075, Japan
(Received 14 October 2015; accepted 24 December 2015; published online 13 January 2016) Undoped n-type BaSi2films were grown on Si(111) by molecular beam epitaxy, and the valence
band (VB) offset at the interface between the BaSi2 and its native oxide was measured by hard
x-ray photoelectron spectroscopy (HAXPES) at room temperature. HAXPES enabled us to investi-gate the electronic states of the buried BaSi2layer non-destructively thanks to its large analysis
depth. We performed the depth-analysis by varying the take-off angle (TOA) of photoelectrons as 15, 30, and 90 with respect to the sample surface and succeeded to obtain the VB spectra of the BaSi2and the native oxide separately. The VB maximum was located at1.0 eV from the Fermi
energy for the BaSi2and4.9 eV for the native oxide. We found that the band bending did not
occur near the native oxide/BaSi2interface. This result was clarified by the fact that the core-level
emission peaks did not shift regardless of TOA (i.e., analysis depth). Thus, the barrier height of the native oxide for the minority-carriers in the undoped n-BaSi2(holes) was determined to be 3.9 eV.
No band bending in the BaSi2close to the interface also suggests that the large minority-carrier
lifetime in undoped n-BaSi2films capped with native oxide is attributed not to the band bending in
the BaSi2, which pushes away photogenerated minority carriers from the defective surface region,
but to the decrease of defective states by the native oxide.VC 2016 AIP Publishing LLC. [http://dx.doi.org/10.1063/1.4939614]
Thin-film solar cells composed of Cu(In,Ga)Se2(CIGS)
and CdTe have yielded practical applications because of their high energy conversion efficiency and low cost.1–6 These materials include toxic and/or not-abundant metal ele-ments. Therefore, materials consisting of earth-abundant and environmental-friendly elements are preferable. To realize such thin-film solar cells, Si thin-film solar cells have been studied extensively;7–12 however, it is not easy to achieve high efficiency as large as 20% because the absorption coef-ficient of crystalline Si is much smaller than that of CIGS. It is thereby very important to explore other thin-film solar cell materials composed of non-toxic and earth abundant ele-ments. Among such materials, we have focused much atten-tion on semiconducting barium disilicide (BaSi2). BaSi2has
a band gap of approximately 1.3 eV, matching the solar spec-trum.13,14 In addition, it has a large absorption coefficient reaching 3 104cm1at 1.5 eV,14which might enable us to
achieve high-efficiency thin-film solar cells. Besides, minority-carrier diffusion length (ca. 10 lm)15and minority-carrier lifetime, s, (ca. 14 ls)16,17 of undoped n-BaSi2 are
sufficiently large for thin-film solar cell application. Our pre-vious studies suggested that the native oxide layer on the sur-face of undoped n-BaSi2 acts as a passivation layer; s
reached approximately 10 ls.18According to the previous x-ray photoelectron spectroscopy (XPS) studies, we found that this native oxide layer was composed of oxides such as SiOx
and BaCO3.18 But we could not discuss how the native
oxides contribute to the surface passivation due to the lack of depth-dependent analysis for the native oxide/n-BaSi2
heter-ostructure. In addition, we have recently achieved the solar cell operation in the devices utilizing the native oxide/n-BaSi2 heterointerface.19 The efficiency was quite limited
because the transport of photogenerated minority carriers (holes) was blocked by the native oxide. In order to improve the device performance, extraction of the photogenerated holes more efficiently through the native oxide layer via tun-neling is needed. At present, the barrier height of the native oxide for holes is unknown. Hard x-ray photoelectron spec-troscopy (HAXPES) is a powerful tool as a direct probe of valence band (VB) density of states (DOS) of BaSi2under its
native oxide. This is because the analysis-depth of HAXPES is much deeper than that of conventional XPS and ultraviolet photoelectron spectroscopy.20–29 In general, conventional XPS in the electron kinetic-energy range of 50–100 eV is quite surface sensitive due to the short electron inelastic mean free path (IMFP), k, of <5 A˚ . The conventional XPS spectra strongly reflect electronic states at surfaces of solids,
which make it difficult to examine the electronic states inside the solids. Although the larger probing depth than 50 A˚ could be expected for HAXPES, a significantly reduced photoioni-zation cross-section prevented us from measuring VB photo-electron spectra above 3 keV.30,31An extremely brilliant X-ray provided from the third generation synchrotron source can well compensate for the diminished cross section and has enabled us to perform HAXPES measurements with high-energy resolution.32 There have been several reports utilizing this large probing depth on the measurement of VB spectra of buried layers such as CdS/Cu2ZnSnS4 (CZTS),
AlOx/Si heterostructures, and Bi2Se3surface.20–22For
exam-ple, in Ref.20, CdS/CZTS heterostructures formed on Mo-coated glass, where the CdS layer thickness was varied as 0, 5, and 100 nm, were examined by changing the effective IMFP, which was controlled by take-off angle (TOA) of pho-toelectrons in HAXPES. Consequently, they succeeded to measure the VB spectra of CdS and CZTS, separately, and obtained the VB offset (VBO) at the CdS/CZTS interface to be 0.0 6 0.1 eV in a real device structure. In this study, we have performed the HAXPES measurements for the native oxide/BaSi2 in order to examine the VBO at the interface,
and the band bending near the interface.
II. EXPERIMENTAL METHOD
We used an ion-pumped molecular beam epitaxy (MBE) system equipped with standard Knudsen cells for Ba and CaF2and an electron-beam evaporation source for Si in this
study. The base pressure of the MBE system was less than 108Pa. The procedure of the sample preparation is as fol-lows. First, Ba was deposited on a Si(111) substrate at 500C to form a 5-nm-thick BaSi2template layer by reactive
deposition epitaxy (RDE).33 This layer works as a kind of seed crystals for subsequent layers. Next, Ba and Si were co-evaporated on the template layer at 580C by MBE to form 600-nm-thick undoped n-BaSi2epitaxial films.34,35After the
MBE growth, the sample was exposed to air for 3 min (sam-ple A) and 24 h (sam(sam-ple B) to form a native oxide on the BaSi2surface, followed by the deposition of a 100-nm-thick
ITO layer by radio-frequency magnetron sputtering method at room temperature (RT). For sample C, the BaSi2surface
was exposed to air for 26 h after the MBE growth. For com-parison, sample D was prepared, where the BaSi2film was
cappedin situ with a 2-nm-thick CaF2layer in order to
pre-vent the surface oxidation.36The oxide layer thicknesses for samples A and B were evaluated by cross-sectional transmis-sion electron microscope (TEM; FEI, Tecnai Osiris) with an acceleration voltage of 200 kV. Thin foils for TEM observa-tion were prepared with a focused ion beam micro-sampling system. The layer structures of samples A–D are summarized in TableI.
HAXPES measurements were performed at the revolver undulator beamline BL15XU32,37of SPring-8 in Japan. The excitation photon energy was set to 5953 eV, and the inci-dent angle of the photon was set to ca. 2–5with respect to the sample surface. The TOA dependence of HAXPES measured at 15, 30, and 90with respect to the sample sur-face was performed at RT. The overall energy resolution was
set to 150 meV. The Fermi energy, EF, was referred to the
Fermi cut-off of an evaporated Au film.
III. RESULTS AND DISCUSSION
Figures 1(a) and 1(b) show the bright-field cross-sec-tional TEM images and the selected area diffraction (SAD) patterns of samples A and B, respectively. As shown in the SAD patterns, diffraction spots corresponding to (200), (400), and (600) planes of BaSi2are aligned normal to the
sample surface, thereby we succeeded to grow the a-axis-ori-ented BaSi2 epitaxial films on Si(111). The native oxide
layer thickness is approximately 6 nm in sample A and 8 nm in sample B. The difference between them is small although the air exposure duration is quite different, that is, 3 min for sample A and 24 h for sample B. This means that the native oxide layer formed in a short period of time, and its layer thickness almost saturated after 24 h. Therefore, it is reasona-ble to suppose the native oxide layer thickness in sample C, used for HAXPES measurements, to be also approximately 8 nm. Regarding the stability and reproducibility of the native oxide, it was found from the secondary ion mass spec-trometry measured on samples more than one month after their growth that a large concentration of O atoms (1022cm3) existed only in the region close to the samples
surface like in samples A and B. We can thereby safely state that the native oxide is stable at least on a BaSi2epitaxial
film during such period.
TABLE I. Sample preparation: BaSi2layer thickness, air exposure duration,
native oxide thickness, and surface capping, and its layer thickness are specified. Sample BaSi2layer (nm) Air exposure duration Native oxide (nm) Capping (nm) A 600 3 min 6 100 (ITO) B 600 24 h 8 100 (ITO) C 600 26 h ca. 8 0 D 35 0 0 2 (CaF2)
FIG. 1. Cross-sectional TEM and SAD images of (a) ITO(100 nm)/oxide (6 nm)/BaSi2(600 nm) (sample A) and (b) ITO(100 nm)/oxide(8 nm)/
BaSi2(600 nm) (sample B).
Figure 2shows the wide range HAXPES spectra of (a) sample C and (b) sample D36taken at TOA¼ 90. In the
fig-ures, we can see the intense peaks of the Ba and Si core-levels. In addition, the O 1s core-level peak was also observed in sam-ple C as seen in Fig.2(a). On the other hand, the O 1s core-level peak was negligibly weak in sample D, which was BaSi2
cappedin situ with CaF2,36in Fig.2(b).
Figure 3(a) shows the expected spectrum, which is the sum of the rescaled partial DOSs of Si 3s, 3p, and Ba 6s states using their photo-ionization cross-sections at a photon energy of 6 keV.EFis located in the middle of the band gap.
Calculation details are given in our previous report.36 The main VB feature of BaSi2 extends from approximately
0.5 eV to 4 eV. The validity of this calculation was proved by the measured VB HAXPES spectrum of sample D in Fig.3(b), which resembles the calculated VB spectrum in Fig.3(a). The contribution of the 2-nm-thick CaF2capping
layer to the VB spectrum was negligible because of the fol-lowing two reasons: (1) the VB maximum of CaF2is located
far below that of BaSi2due to the large band gap (ca. 12 eV),
and (2) the spectrum in Fig. 3(b) was not measured under surface-sensitive condition but under bulk-sensitive condi-tion. According to Tanuma-Powell-Penn equation,38 the IMFP value, k, was calculated to be approximately 10 nm for BaSi2 at 6 keV. The HAXPES intensity decays as
exp(x/k) at a depth x beneath the surface, and the photo-electron which contributes to the HAXPES intensity comes from a range of 3k from the surface. Thus, the probing depth is estimated to be 3k sin(TOA), that is, approximately 30 nm for TOA¼ 90. This value is much larger than the
native oxide layer thickness (ca. 8 nm), and therefore, the HAXPES intensity originating from the BaSi2becomes
pro-nounced. For these reasons, the contribution of the CaF2can
be neglected in Fig.3(b).
Next, we discuss the results on sample C, BaSi2capped
with native oxide. Figures3(c)–3(e)show the HAXPES spec-tra measured at TOA¼ 90, 30, and 15, respectively. The
spectrum in Fig.3(c)was measured under bulk-sensitive con-dition and that in Fig.3(e)under surface-sensitive condition. The VB HAXPES spectrum in Fig. 3(c) is quite similar to that in Fig. 3(b). The VB structures originating from the BaSi2start to increase at approximately1 eV and extend up
to approximately 4 eV in sample C, measured at TOA¼ 90. On the other hand, the VB structures are
negligi-bly weak in the above-mentioned energy range at TOA¼ 15
as shown in Fig. 3(e). We should also note that the VB HAXPES spectrum in Fig. 3(d) is the intermediate one between those in Figs. 3(c) and 3(e). Since the HAXPES spectrum shown in Fig.3(e)was measured under the surface-sensitive condition of TOA¼ 15, it is safe to state that the
VB of the native oxide appears dominant in Fig.3(e). Figures4(a)and4(b), respectively, show the HAXPES spectrum around 1.0 eV in Fig. 3(c), near the VB maxi-mum of BaSi2,EBaSi2V , and that around5.0 eV in Fig.3(e),
near the VB maximum of the native oxide,Eoxide V .E
BaSi2 V and
EoxideV are derived to be1.0 and 4.9 eV, respectively, with
respect to EF by means of the linear extrapolation to the
baseline as shown in Fig.4. VBO at the native oxide/BaSi2
is not given just by the difference between EoxideV andE BaSi2 V
because the band bending in the BaSi2 near the interface
should be considered. To investigate the influence of this band bending, we next compared the core-level spectra obtained for different TOAs.
Figure5shows the Ba 3d3/2core-level spectra in sample
C at TOA¼ 15, 30, and 90. Each spectrum is well
recon-structed by the sum of two Gaussian curves (broken lines) located at795.9 eV and 797.1 eV. We attribute the peak at 795.9 eV (797.1 eV) to the BaSi2 layer (the surface
native oxide layer) because of the strong reduction of the
FIG. 2. Wide-range HAXPES spectra of (a) oxide(ca. 8 nm)/BaSi2(600 nm)
(sample C) and (b) CaF2(2 nm)/BaSi2(35 nm) (sample D).36
FIG. 3. (a) Calculated spectrum36 and (b) HAXPES spectrum of
CaF2(2 nm)/BaSi2(35 nm) (sample D).36 HAXPES spectra of oxide(ca.
8 nm)/BaSi2(600 nm) (sample C) when TOA is (c) 90, (d) 30, and (e) 15.
peak at 795.9 eV in the surface-sensitive spectrum (TOA¼ 15). As seen in Fig. 5, the peak energy positions
and shapes did not change regardless of TOA, thereby ana-lyzing depth information. This means that the band bending did not occur or it was negligibly small around the oxide/ BaSi2interface. If there are lot of defects in the BaSi2close
to the interface,EFpinning is likely to occur there, resulting
in the band bending as is often the case with Si,39GaAs,40 and InN.41No band bending in the BaSi2layer indicates that
the native oxide/BaSi2interface is not defective. This is
con-sistent with our previous result.19According to Ref.19, the capacitance versus voltage characteristics of the device structures composed of the native oxide/BaSi2 interface
revealed that the trapped electrons at the surface defect states decreased with the air exposure duration of the BaSi2
surface. On the basis of these results, the band lineup of the native oxide layer and BaSi2can be obtained as shown in
Fig.6. We thus conclude that the barrier height of the native oxide layer against holes, minority carriers in n-BaSi2, is
approximately 3.9 eV (¼ 4.9 eV – 1.0 eV).
We next discuss the reason why the minority-carrier lifetime in undoped n-type BaSi2is improved from ca. 0.2 ls
to ca. 10 ls by forming the native oxide on the BaSi2
sur-face.18Surface passivation is widely known in crystalline Si capped with oxides such as SiO2and Al2O3.
It is attrib-uted to two mechanisms, that is, the decrease of surface states in Si by terminating the dangling bonds of Si and the electric-field due to charges in the oxides, which bends the energy band of Si near the oxide/Si interface so as the photogenerated minority carriers are pushed away from the defective surface region. In the case of native oxide/BaSi2,
such a band bending does not exist as discussed in Fig.5. It is thus the decrease of the surface states that accounts for the large minority-carrier lifetime obtained for BaSi2 capped
with native oxide. Now that the barrier height of holes is made clear, and thinning of the oxide layer thickness with more precision might enhance the transport of photogener-ated holes through the native oxide layer via tunneling and improve the solar cell efficiency much further.
We formed 600-nm-thick a-axis-oriented undoped n-BaSi2 epitaxial layers on Si(111) by MBE and directly
measured the electronic states of the buried BaSi2 layers
under the 8-nm-thick native oxide by HAXPES. We per-formed the depth-analysis by varying TOA of 15, 30, and 90and obtained the VB spectra of the BaSi2and the native
oxide separately. The VB maximum was located at4.9 eV fromEFfor the native oxide and1.0 eV for the BaSi2. The
VBO at the native oxide/BaSi2interface, that is, the barrier
height for holes in n-BaSi2, was thus determined to be
3.9 eV. The Ba 3d core-level HAXPES spectra revealed that there was no band bending in the BaSi2close to the native
oxide/BaSi2 interface. This means that the large
minority-carrier lifetime in undoped n-BaSi2films capped with native
FIG. 4. Enlarged spectra for sample C around (a)1 eV in Fig.3(c)and 3(b)5 eV in Fig.3(e), corresponding to the HAXPES spectra around the VB maximum of BaSi2and native oxide, respectively.
FIG. 5. Ba 3d3/2 core-level HAXPES spectra for sample C taken at
TOA¼ 15, 30, and 90. Each spectrum can be fitted by the sum of two
Gaussian curves (broken lines) peaking at 795.9 eV and 797.1 eV. Broken lines are shifted downward a little to be seen.
FIG. 6. Band lineup of the native oxide and BaSi2layers determined by the
oxide is attributed not to the band bending in the BaSi2,
which keeps photogenerated minority carriers away from the defective surface region, but to the decrease of defective states by the native oxide.
The HAXPES measurements were performed at Synchrotron X-ray Station of BL15XU, at SPring-8, and were supported by NIMS microstructural characterization platform as a program of “Nanotechnology Platform” (Proposal Nos. 2014A4902 and 2015A4907) of the Ministry of Education, Culture, Sports, Science and Technology (MEXT), Japan. S.U and A.K. are grateful to HiSOR, Hiroshima University and JAEA at SPring-8 for the development of HAXPES at BL15XU. The authors thank Dr. N. Yoshizawa and Mr. N. Saito for their help in TEM observations conducted at the Electron Microscope Facility, supported by the IBEC Innovation Platform, AIST, Japan. This work was financially supported by the Japan Science and Technology Agency (JST/CREST) and by a Grants-in-Aid for Scientific Research A (15H02237) from the Japan Society for the Promotion of Science (JSPS). R.T. was financially supported by Grants-in-Aid for JSPS Fellows (15J02139).
A. Romeo, A. Terheggen, D. Abou-Ras, D. L. Batzner, F. J. Haug, M. Kalin, D. Rudmann, and A. N. Tiwari,Prog. Photovoltaics12, 93 (2004).
2I. Repins, M. A. Contreras, B. Egaas, C. DeHart, J. Scharf, C. L. Perkins,
B. To, and R. Noufi,Prog. Photovoltaics16, 235 (2008).
M. A. Green and S. R. Wenham,Appl. Phys. Lett.65, 2907 (1994).
4H. Katagiri, K. Jimbo, W. S. Maw, K. Oishi, M. Yamazaki, H. Araki, and
A. Takeuchi,Thin Solid Films517, 2455 (2009).
K. Tanaka, M. Oonuki, N. Moritake, and H. Uchiki,Sol. Energy Mater. Sol. Cells93, 583 (2009).
6W. W. Yu, L. Qu, W. Guo, and X. Peng,Chem. Mater.15, 2854 (2003). 7H. Sasaki, H. Morikawa, Y. Matsuno, M. Deguchi, T. Ishihara, H. Kumabe,
T. Murotani, and S. Mitsui,Jpn. J. Appl. Phys., Part 133, 3389 (1994).
J. Meier, S. Dubail, R. Platz, P. Torres, U. Kroll, J. A. A. Selvan, N. P. Vaucher, Ch. Hof, D. Fischer, H. Keppner, R. Fl€uckiger, A. Shah, V. Shklover, and K.-D. Ufert,Sol. Energy Mater. Sol. Cells49, 35 (1997).
O. Vetterl, F. Finger, R. Carius, P. Hapke, L. Houben, O. Kluth, A. Lambertz, A. M€uck, B. Rech, and H. Wagner,Sol. Energy Mater. Sol. Cells62, 97 (2000).
10J. M€uller, B. Rech, J. Springer, and M. Vanecek,Sol. Energy
77, 917 (2004).
A. V. Shah, H. Schade, M. Vanecek, J. Meier, E. Vallat-Sauvain, N. Wyrsch, U. Kroll, C. Droz, and J. Bailat,Prog. Photovoltaics12, 113 (2004).
P. Bermel, C. Luo, L. Zeng, L. C. Kimerling, and J. D. Joannopoulus,Opt. Express15, 16986 (2007).
K. Morita, Y. Inomata, and T. Suemasu, Thin Solid Films 508, 363 (2006).
14K. Toh, T. Saito, and T. Suemasu,Jpn. J. Appl. Phys., Part 1
50, 068001 (2011).
M. Baba, K. Toh, K. Toko, N. Saito, N. Yoshizawa, K. Jiptner, T. Sakiguchi, K. O. Hara, N. Usami, and T. Suemasu,J. Cryst. Growth348, 75 (2012).
K. O. Hara, N. Usami, K. Toh, M. Baba, K. Toko, and T. Suemasu, J. Appl. Phys.112, 083108 (2012).
17K. O. Hara, N. Usami, K. Nakamura, R. Takabe, M. Baba, K. Toko, and T.
Suemasu,Appl. Phys. Express6, 112302 (2013).
R. Takabe, K. O. Hara, M. Baba, W. Du, N. Shimada, K. Toko, N. Usami, and T. Suemasu,J. Appl. Phys.115, 193510 (2014).
19W. Du, R. Takabe, M. Baba, H. Takeuchi, K. O. Hara, K. Toko, N. Usami,
and T. Suemasu,Appl. Phys. Lett.106, 122104 (2015).
S. Tajima, K. Kataoka, N. Takahashi, Y. Kimoto, T. Fukano, M. Hasegawa, and H. Hazama,Appl. Phys. Lett.103, 243906 (2013).
21N. Ikeno, Y. Yamashita, H. Oji, S. Miki, K. Arafune, H. Yoshida, S.
Satoh, I. Hirosawa, T. Chikyow, and A. Ogura,Jpn. J. Appl. Phys., Part 1 54, 08KD19 (2015).
C. E. ViolBarbosa, C. Shekhar, B. Yan, S. Ouardi, E. Ikenaga, G. H. Fecher, and C. Felser,Phys. Rev. B88, 195128 (2013).
M. Sowinska, T. Bertaud, D. Walczyk, S. Thiess, M. A. Schubert, M. Lukosius, W. Drube, Ch. Walczyk, and T. Schoeder,Appl. Phys. Lett. 100, 233509 (2012).
24J. Rubio-Zuazo and G. R. Castro,Surf. Interface Anal.
40, 1438 (2008).
R. Claessen, M. Sing, M. Paul, G. Berner, A. Wetscherek, A. M€uller, and W. Drube,New J. Phys.11, 125007 (2009).
26G. Panaccione and K. Kobayashi,Surf. Sci.606, 125 (2012).
27T. Nagata, S. Oh, Y. Yamashita, H. Yoshikawa, N. Ikeno, K. Kobayashi,
T. Chikyow, and Y. Wakayama,Appl. Phys. Lett.102, 043302 (2013).
L. A. Walsh, G. Hughes, P. K. Hurley, J. Lin, and J. C. Woicik, Appl. Phys. Lett.101, 241602 (2012).
D. Gerlach, R. G. Wilks, D. Wippler, M. Wimmer, M. Lozac’h, R. Felix, A. M€uck, M. Meier, S. Ueda, H. Yoshikawa, M. Gorgoi, K. Lips, B. Rech, M. Sumiya, J. H€upkes, K. Kobayashi, and M. B€ar,Appl. Phys. Lett.103, 023903 (2013).
M. B. Trzhaskovskaya, V. I. Nefedov, and V. G. Yarzhemsky,At. Data Nucl. Data Tables77, 97 (2001).
31M. B. Trzhaskovskaya, V. I. Nefedov, and V. G. Yarzhemsky,At. Data
Nucl. Data Tables82, 257 (2002).
S. Ueda, Y. Katsuya, M. Tanaka, H. Yoshikawa, Y. Yamashita, S. Ishimaru, Y. Matsushita, and K. Kobayashi,AIP Conf. Proc.1234, 403 (2010).
33Y. Inomata, T. Nakamura, T. Suemasu, and F. Hasegawa, Jpn. J. Appl.
Phys., Part 143, 4155 (2004).
Y. Inomata, T. Nakamura, T. Suemasu, and F. Hasegawa, Jpn. J. Appl. Phys., Part 243, L478 (2004).
35R. Takabe, K. Nakamura, M. Baba, W. Du, M. A. Khan, K. Toko, M.
Sasase, K. O. Hara, N. Usami, and T. Suemasu, Jpn. J. Appl. Phys.53, 04ER04 (2014).
36M. Baba, K. Ito, W. Du, T. Sanai, K. Okamoto, K. Toko, S. Ueda, Y. Imai,
A. Kimura, and T. Suemasu,J. Appl. Phys.114, 123702 (2013).
S. Ueda,J. Electron Spectrosc. Rel. Phenom.190, 235 (2013).
S. Tanuma, C. J. Powell, and D. R. Penn,Surf. Interface Anal.43, 689 (2011).
F. J. Himpsel, G. Hollinger, and R. A. Pollak, Phys. Rev. B28, 7014 (1983).
H. Hasegawa, H. Ishi, T. Sawada, T. Saitoh, S. Konishi, Y. Liu, and H. Ohno,J. Vac. Technol. B6, 1184 (1988).
I. Mahboob, T. D. Veal, C. F. McConville, H. Lu, and W. J. Schaff,Phys. Rev. Lett.92, 036804 (2004).
42A. G. Aberle, S. Glunz, and W. Warta,J. Appl. Phys.71, 4422 (1992). 43A. W. Stephens, A. G. Aberle, and M. A. Green,J. Appl. Phys.76, 363
S. W. Glunz, A. B. Sproul, W. Warta, and W. Wettling,J. Appl. Phys.75, 1611 (1994).
45H. Kobayashi, A. Asano, S. Asada, T. Kubota, Y. Yamashita, K. Yoneda,
and Y. Todoroki,J. Appl. Phys.83, 2098 (1998).
A. G. Aberle,Prog. Photovoltaics8, 473 (2000).
47B. Hoex, S. B. S. Heil, E. Langereis, M. C. M. van de Sanden, and W. M.
M. Kessels,Appl. Phys. Lett.89, 042112 (2006).
J. Schmidt, A. Merkle, R. Brendel, B. Hoex, M. C. M. van de Sanden, and W. M. M. Kessels,Prog. Photovoltaics16, 461 (2008).